Polycrystal Plasticity - Multiple Slip

# Polycrystal Plasticity - Multiple Slip

Télécharger la présentation

## Polycrystal Plasticity - Multiple Slip

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -
##### Presentation Transcript

1. Polycrystal Plasticity -Multiple Slip 27-750 Texture, Microstructure & Anisotropy A.D. Rollett, H. Garmestani (GaTech), G. Branco (FAMU/FSU) Last revised:14th Aug. 2012

2. Objective • The objective of this lecture is to show how plastic deformation in polycrystals requires multiple slip in each grain. • Further, to show how to calculate the distribution of slips in each grain of a polycrystal (principles of operation of Los Alamos polycrystal plasticity, LApp; also the Viscoplastic Selfconsistent code, VPSC). Requirements: • Dislocation controlled plastic strain • Mechanics of Materials • Continuum Mechanics

3. Questions • What is the difference between single slip and multiple slip in terms of boundary conditions? • What is “deviatoric stress” and why does it have 5 components? • How does the von Mises criterion for ductility relate to the 5 components of deviatoric stress and strain? • How does the Bishop-Hill theory work? What is the input and output to the algorithm? What is meant by the “maximum work” principle? • What is the Taylor factor (both definition and physical meaning)? • Why is the rate-sensitive formulation for multiple slip useful above and beyond what the Bishop-Hill approach gives? • What is it that causes/controls texture development? • On what quantities is lattice reorientation based (during multiple slip)? • How can we compute the macroscopic strain due to any given slip system? • How can we compute the resolved shear stress on a given slip system, starting with the macroscopic stress (tensor)? • What does Bishop & Hill state of stress mean (what is the physical meaning)? [Each B&H stress state (one of the 28) corresponds to a corner of the single xtal yield surface that activates either 6 or 8 slip systems simultaeneously]

4. References • Kocks, Tomé & Wenk: Texture & Anisotropy (Cambridge); chapter 8, 1996. Detailed analysis of plastic deformation and texture development. • Reid: Deformation Geometry for Materials Scientists, 1973. Older text with many nice worked examples. Be careful of his examples of calculation of Taylor factor because, like Bunge & others, he does not use von Mises equivalent stress/strain to obtain a scalar value from a multiaxial stress/strain state. • Hosford: The Mechanics of Crystals and Textured Polycrystals, 1993 (Oxford). Written from the perspective of a mechanical metallurgist with decades of experimental and analytical experience in the area. • Khan & Huang: Continuum Theory of Plasticity. Written from the perspective of continuum mechanics. • De Souza Neto, Peric & Owen: Computational Methods for Plasticity, 2008 (Wiley).Written from the perspective of continuum mechanics. • Key Papers: Taylor G., (1938) Plastic strain in metals, J. Inst. Metals (U.K.) 62 307 ; Bishop J and Hill R (1951) Phil. Mag. 42 1298.

5. Background, Concepts

6. Increasing strain Output of LApp • Figure shows pole figures for a simulation of the development of rolling texture in an fcc metal. • Top = 0.25 von Mises equivalent strain; 0.50, 0.75, 1.50 (bottom). • Note the increasing texture strength as the strain level increases.

7. Development The Theory depends upon: • The physics of single crystal plastic deformation; • relations between macroscopic and microscopic quantities ( strain, stress ...); The mathematical representation and models • Initially proposed by Sachs (1928), Cox and Sopwith (1937), and Taylor in 1938. Elaborated by Bishop and Hill (1951), , Kocks, Asaro& Needleman, Canova. • Self-Consistent model by Kröner (1958, 1961), extended by Budiansky and Wu (1962). • Further developments by Hill (1965a,b) and Lin (1966, 1974, 1984) and others. • Read Taylor (1938) “Plastic strain in metals.” J. Inst. Metals (U.K.) 62, 307. - available as: Taylor.1938.pdf

8. Sachs versus Taylor Sachs Model (previous lecture on single crystal): • All single-crystal grains with aggregate or polycrystal experience the same state of stress; • Equilibrium condition across the grain boundaries satisfied; • Compatibility conditions between the grains violated, thus, finite strains will lead to gaps and overlaps between grains; • Generally most successful for single crystal deformation with stress boundary conditions on each grain. Taylor Model (this lecture): • All single-crystal grains within the aggregate experience the same state of deformation (strain); • Equilibrium condition across the grain boundaries violated, because the vertex stress states required to activate multiple slip in each grain vary from grain to grain; • Compatibility conditions between the grains satisfied; • Generally most successful for polycrystals with strain boundary conditions on each grain.

9. Sachs versus Taylor: 2 • Diagrams illustrate the difference between the Sachs iso-stress assumption of single slip in each grain (a, c and e) versus the Taylor assumption of iso-strain with multiple slip in each grain (b, d). iso-stress iso-strain

10. Sachs versus Taylor: 3 Single versus Multiple Slip External Stress or External Strain Small arrows indicate variable stress state in each grain Small arrows indicate identical stress state in each grain Multiple slip (with 5 or more systems) in each grain satisfies the externally imposed strain, D Increasing strain Each grain deforms according to which single slip system is active D = ETd

11. Taylor model: uniform strain An essential assumption of the Taylor model is that each grain conforms to the macroscopic strain imposed on the polycrystal

12. Example of Slip Lines at Surface (plane strain stretched Al 6022) T-Sample at 15% strain • Note how each grain exhibits varying degrees of slip line markings. • Although any given grain has one dominant slip line (trace of a slip plane), more than one is generally present. • Taken from PhD research of Yoon-Suk Choi on surface roughness development in Al 6022 PD // TD PSD // RD

13. Notation: 1 • Strain, local: Elocal; global: Eglobal • Slip direction (unit vector): b or s • Slip plane (unit) normal: n • Slip tensor, mij = binj =Pij • Stress (tensor or vector): s • Shear stress (usually on a slip system): t • Shear strain (usually on a slip system): g • Stress deviator (tensor): S • Rate sensitivity exponent: n • Slip system index: sor  • Note that when an index (e.g. of a Slip system, b(s)n(s)) is enclosed in parentheses, it means that the summation convention does not apply even if the index is repeated in the equation.

14. Notation: 2 • Coordinates: current: x; reference X • Velocity of a point: v. • Displacement: u • Hardening coefficient: h (ds h dg • Strain, e • measures the change in shape • Work increment: dW • do not confuse with spin! • Infinitesimal rotation tensor: W • Elastic Stiffness Tensor (4th rank): C • Load, e.g. on a tensile sample: P • do not confuse with slip tensor!

15. Notation: 3 • Plastic spin: W • measures the rotation rate; more than one kind of spin is used: • “Rigid body” spin of the whole polycrystal: W • “grain spin”of the grain axes (e.g. in torsion): Wg • “lattice spin” from slip/twinning (skew symmetric part of the strain): Wc. • Rotation (small): w

16. Notation: 4 • Deformation gradient: F • Measures the total change in shape (rotations included). • Velocity gradient: L • Tensor, measures the rate of change of the deformation gradient • Time: t • Slip geometry matrix: E (do not confuse with strain) • Strain rate: D • symmetric tensor;D = symm(L)

17. Schmid / Sachs / Single Slip

18. Schmid’s Law • Initial yield stress varies from sample to sample depending on, among several factors, the relation between the crystal lattice to the loading axis (i.e. orientation, written as g). • The applied stress resolved along the slip direction on the slip plane (to give a shear stress) initiates and controls the extent of plastic deformation. • Yield begins on a given slip system when the shear stress on this system reaches a critical value, called the critical resolved shear stress (crss), independent of the tensile stress or any other normal stress on the lattice plane (in less symmetric lattices, however, there may be some dependence on the hydrostatic stress). • The magnitude of the yield stress depends on the density and arrangement of obstacles to dislocation flow, such as precipitates (not discussed here).

19. Minimum Work, Single Slip (Sachs) Under stress boundary conditions, single slip occurs Uniaxial Tension or Compression (where “m” is the slip tensor): = n The (dislocation) slip is given by (where “m” is the Schmid factor): = b,or, s P is a unit vector in the loading direction This slide, and the next one, are a re-cap of the lecture on single slip

20. Minimum Work, Single Slip Applying the Minimum Work Principle, it follows that Note: t(g) describes the dependence of the critical resolved shear stress (crss) on strain (or slip curve), based on the idea that the crssincreases with increasing strain. The Schmid factor,m, has a maximum value of 0.5 (both angles = 45°).

21. Dislocations, Slip Systems, Crystallography

22. Dislocations and Plastic Flow • At room temperature the dominant mechanism of plastic deformation is dislocation motion through the crystal lattice. • Dislocation glide occurs on certain crystal planes (slip planes) in certain crystallographic directions (// Burgers vector). • A slip system is a combination of a slip direction and slip plane normal. • A second-rank tensor (mij = binj) can associated with each slip system, formed from the outer product of slip direction and normal. The resolved shear stress on a slip system is then given by  mijij. • The crystal structure of metals is not altered by the plastic flow because slip is a simple shear mode of deformation. Moreover no volume change is associated with slip, therefore the hydrostatic stress has no effect on plasticity (in the absence of voids). This explains the use of deviatoric stress in calculations.

23. Crystallography of Slip Slip occurs most readily in specific directions on certain crystallographic planes. Slip plane – is the plane of greatest atomic density. Slip direction – is the close-packed direction within the slip plane. Slip system – is the combination of preferred slip planes and slip directions (on those specific planes) along which dislocation motion occurs. Slip systems are dependent on the crystal structure.

24. Crystallography of Slip in fcc Example: Determine the slip system for the (111) plane in a fcc crystal and sketch the result. The slip direction in fcc is <110> The proof that a slip direction [uvw] lies in the slip plane (hkl) is given by calculating the scalar product: hu + kv + lw =0

25. Slip Systems in fcc, bcc, hcp The slip systems for FCC, BCC and HCP crystals are For this lecture we will focus on FCC crystals only Note: In the case of FCC crystals we can see in the table that there are 12 slip systems. However if forward and reverse systems are treated as independent, there are then 24 slip systems.

26. Elastic vs. Plastic Deformation Selection of Slip Systems for Rigid-Plastic Models Assumption – For FPD, the elastic deformation rate is usually small when compared to the plastic deformation rate and thus it can be neglected. Reasons: Perfect plastic materials - equivalent stress = initial yield stress The elastic deformation is confined to the ratio of stress to elastic modulus For most metals – initial yield stress is 2 or 3 orders of magnitude less than the elastic modulus – ratio is << 1

27. Macro Strain – Micro Slip Selection of Slip Systems for Rigid-Plastic Models Once the elastic deformation rate is considered, it is reasonable to model the material behavior using the rigid-plastic model given by: where forward and reverse considered independent n is ≤ to 12 systems (or 24 systems – ) Note: D can expressed by six components ( Symmetric Tensor) Because of the condition - , only five out of the six components are independent.

28. Von Mises criterion Selection of Slip Systems for Rigid Plasticity Models As a consequence of the condition the number of possible active slip systems (in cubic metals) is greater than the number of independent components of the tensor strain rate Dp, from the mathematical point of view (under-determined system), so any combination of five slip systems that satisfy the incompressibility condition can allow the prescribed deformation to take place. The requirement that at least five independent systems are required for plastic deformation is known as the von Mises Criterion. If less than 5 independent slip systems are available, the ductility is predicted to be low in the material. The reason is that each grain will not be able to deform with the body and gaps will open up, i.e. it will crack. Caution: even if a material has 5 or more independent systems, it may still be brittle (e.g. Iridium).

29. Minimum Work Principle • Proposed by Taylor in (1938). • The objective is to determine the combination of shears or slips that will occur when a prescribed strain is produced. • States that, of all possible combinations of the 12 shears that can produce the assigned strain, only that combination for which the energy dissipation is the least is operative. • The defect in the approach is that it says nothing about the activity or resolved stress on other, non-active systems (This last point was addressed by Bishop and Hill in 1951). Mathematical statement: Bishop J and Hill R (1951) Phil. Mag. 42 1298

30. Minimum Work Principle Minimum Work Principle Here, - are the actually activated slips that produce D. - is any set of slips that satisfy tr(D)=Dii = 0, but are operated by the corresponding stress satisfying the loading/unloading criteria. - is the (current) critical resolved shear stress (crss) for the material (applies on any of the th activated slip systems). - is the current shear strength of (= resolved shear stress on) the th geometrically possible slip system that may not be compatible with the externally applied stress.

31. Minimum Work Principle Recall that in the Taylor model all the slip systems are assumed to harden at the same rate, which means that and then, Note that, now, we have only 12 operative slip systems once the forward and reverse shear strengths (crss) are considered to be the same in absolute value.

32. Minimum Work Principle Thus Taylor’s minimum work criterion can be summarized as in the following: Of the possible 12 slip systems, only that combination for which the sum of the absolute values of shears is the least is the combination that is actually operative! The uniformity of the crss means that the minimum work principle is equivalent to a minimum microscopic shear principle.

33. Stress > CRSS? • The obvious question is, if we can find a set of microscopic shear rates that satisfy the imposed strain, how can we be sure that the shear stress on the other, inactive systems is not greater than the critical resolved shear stress? • This is not the same question as that of equivalence between the minimum work principle and the maximum work approach described later in this lecture.

34. Stress > CRSS? • The work increment is the (inner) product of the stress and strain tensors, and must be the same, regardless of whether it is calculated from the macroscopic quantities or the microscopic quantities:For the actual set of shears in the material, we can write (omitting the “*”),where the crss is outside the sum because it is constant. [Reid: pp 154-156]

35. Stress > CRSS? • Now we know that the shear stresses on the hypothetical (denoted by “*”) set of systems must be less than or equal to the crss, tc, for all systems, so:This means that we can write:

36. Stress > CRSS? • However the LHS of this equation is equal to the work increment for any possible combination of slips,dw=sijdeijwhich is equal totc Sdg, leaving us with:So dividing both sides by tcallows us to write: Q.E.D.

37. MultipleSlip

38. MultipleSlip • Deformation rate is multi-axial General case – D • Only five independent (deviatoric) components Crystal - FCC Slip rates - , , ...., ontheslip systems a1, a2, a3 ..., respectively. Note correction to system b2

39. Multiple Slip Using the following set of relations can be obtained Note: ex, ey, ez are unit vectors parallel to the axes TO BE CONTINUED

40. Multiple Slip

41. Multiple Slip To verify these relations, consider the contribution of shear on system c3 as an example: Slip system - c3; Given : Unit vector in the slip direction – Unit normal vector to the slip plane – The contribution of the c3 system is given by

42. Multiple Slip From the set of equations, one can obtain 6relations between the components of D and the 12 shear rates on the 12 slip systems. By taking account of the incompressibility condition, this reduces to only 5 independent relations that can be obtained from the equations. So, the main task is to determine which combination of 5 independent shear rates, out of 12 possible rates, should be chosen as the solution of a prescribed deformation rateD. This set of shear rates must satisfy Taylor’s minimum shear principle. Note : There are 792 sets or 12C5 combinations, of 5 shears, but only 96 are independent. Taylor’s minimum shear principle does not ensure that there is a unique solution (a unique set of 5 shears).

43. Multiple Slip: Strain • Suppose that we have 5 slip systems that are providing the external slip, D. • Let’s make a vector, Di, of the (external) strain tensor components and write down a set of equations for the components in terms of the microscopic shear rates, d. • Set D2 = d22, D3 = d33, D6 = d12, D5 = d13, and D4 = d23. D_2& = [m_{22}^{(1) } & m_{22}^{(2)} & m_{22}^{(3)} & m_{22}^{(4)} & m_{22}^{(5)} ] \cdot [ d\gamma_1& \\ d\gamma_2& \\ d\gamma_3& \\ d\gamma_4& \\ d\gamma_5& ]

44. Multiple Slip: Strain • This notation can obviously be simplified and all five components included by writing it in tabular or matrix form (where the slip system indices are preserved as superscripts in the 5x5 matrix): or, D = ETd \begin{bmatrix} D_2& \\ D_3& \\ D_4& \\ D_5& \\ D_6& \end{bmatrix} = \begin{bmatrix} m_{22}^{(1) } & m_{22}^{(2)} & m_{22}^{(3)} & m_{22}^{(4)} & m_{22}^{(5)} \\ m_{33}^{(1)} & m_{33}^{(2)} & m_{33}^{(3)} & m_{33}^{(4)} & m_{33}^{(5)} \\ (m_{23}^{(1)}+m_{32}^{(1)}) & (m_{23}^{(2)}+m_{32}^{(2)}) & (m_{23}^{(3)}+m_{32}^{(3)}) & (m_{23}^{(4)}+m_{32}^{(4)}) & (m_{23}^{(5)}+m_{32}^{(5)}) \\ (m_{13}^{(1)}+m_{31}^{(1)}) & (m_{13}^{(2)}+m_{31}^{(2)}) & (m_{13}^{(3)}+m_{31}^{(3)}) & (m_{13}^{(4)}+m_{31}^{(4)}) & (m_{13}^{(5)}+m_{31}^{(5)}) \\ (m_{12}^{(1)}+m_{21}^{(1)}) & (m_{12}^{(2)}+m_{21}^{(2)}) & (m_{12}^{(3)}+m_{21}^{(3)}) & (m_{12}^{(4)}+m_{21}^{(4)}) & (m_{12}^{(5)} +m_{21}^{(5)})\end{bmatrix} \begin{bmatrix} d\gamma_1& \\ d\gamma_2& \\ d\gamma_3& \\ d\gamma_4& \\ d\gamma_5& \end{bmatrix}

45. Multiple Slip: Stress • We can perform the equivalent analysis for stress: just as we can form an external strain component as the sum over the contributions from the individual slip rates, so too we can form the resolved shear stress as the sum over all the contributions from the external stress components (note the inversion of the relationship): Or,

46. Multiple Slip: Stress • Putting into 5x6 matrix form, as for the strain components, yields:

47. Definitions of Stress states, slip systems • Now define a set of six deviatoric stress terms, since we know that the hydrostatic component is irrelevant, of which we will actually use only 5:A:= (s22 - s33) F:= s23B:= (s33 - s11) G:= s13C:= (s11 - s22) H:= s12 • Slip systems (as before): Note: these systems have the negatives of the slip directions compared to those shown in the lecture on Single Slip (taken from Khans’ book), except for b2. Kocks: UQ -UK UP -PK -PQ PU -QU -QP -QK -KP -KU KQ

48. Multiple Slip: Stress • Equivalent 5x5 matrix form for the stresses: • Transpose the matrix:

49. Multiple Slip: Stress/Strain Comparison • The last matrix equation is in the same form as for the strain components. • We can test for the availability of a solution by calculating the determinant of the “E” matrix, as in: = ETor, D = ETd • A non-zero determinant means that a solution is available. • Even more important, the direct form of the stress equation means that, if we assume a fixed critical resolved shear stress, then we can compute all the possible multislip stress states, based on the set of linearly independent combinations of slip:= E  • It must be the case that, of the 96 sets of 5 independent slip systems, the stress states computed from them collapse down to only the 28 found by Bishop & Hill.